#------------------------------------------------------------------------------
#$Date: 2019-11-24 08:25:55 +0100 (dom 24 de nov de 2019) $
#$Revision: 237458 $
#$URL: svn://www.crystallography.net/cod/cif/7/23/71/7237156.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7237156
loop_
_publ_author_name
'Dalinger, Igor L.'
'Suponitsky, Kyrill Yu.'
'Shkineva, Tatyana K.'
'Lempert, David B.'
'Sheremetev, Aleksei B.'
_publ_section_title
;
 Bipyrazole bearing ten nitro groups -- a novel highly dense oxidizer for
 forward-looking rocket propulsions
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry A'
_journal_page_first              14780
_journal_paper_doi               10.1039/C8TA05179H
_journal_volume                  6
_journal_year                    2018
_chemical_formula_moiety         'C8 N14 O20'
_chemical_formula_sum            'C8 N14 O20'
_chemical_formula_weight         612.22
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014/6
_audit_update_record
;
2018-04-30 deposited with the CCDC.
2018-07-03 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 91.071(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.9011(13)
_cell_length_b                   10.5386(13)
_cell_length_c                   19.291(2)
_cell_measurement_reflns_used    2140
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      23.47
_cell_measurement_theta_min      2.20
_cell_volume                     2012.5(4)
_computing_cell_refinement       'SAINT (Bruker, 2009)'
_computing_data_collection       'APEX (Bruker, 2009)'
_computing_data_reduction        'SAINT (Bruker, 2009)'
_computing_molecular_graphics    'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_publication_material
'SHELXL-2014/6 (Sheldrick, 2014) and PLATON (Spek, 2009)'
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/6 (Sheldrick, 2014)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0471
_diffrn_reflns_av_unetI/netI     0.0370
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            24502
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.017
_diffrn_reflns_theta_min         2.112
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    0.202
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            pale-yellow
_exptl_crystal_density_diffrn    2.021
_exptl_crystal_description       prizm
_exptl_crystal_F_000             1224
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.16
_refine_diff_density_max         0.304
_refine_diff_density_min         -0.236
_refine_diff_density_rms         0.055
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.033
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     379
_refine_ls_number_reflns         5351
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.033
_refine_ls_R_factor_all          0.0781
_refine_ls_R_factor_gt           0.0462
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0541P)²+0.6302P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1105
_refine_ls_wR_factor_ref         0.1302
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3450
_reflns_number_total             5351
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c8ta05179h2.cif
_cod_data_source_block           rt312
_cod_original_cell_volume        2012.6(4)
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               7237156
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelxl_version_number           2014/6
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
O1 O 0.44344(18) -0.01476(17) 0.65847(9) 0.0575(5) Uani 1 1 d
O2 O 0.27932(16) 0.05004(17) 0.72097(10) 0.0566(4) Uani 1 1 d
O3 O 0.66299(19) -0.07895(18) 0.75361(11) 0.0682(5) Uani 1 1 d
O4 O 0.70444(17) 0.1121(2) 0.71982(9) 0.0640(5) Uani 1 1 d
O5 O 0.5325(2) 0.02303(15) 0.88138(8) 0.0548(4) Uani 1 1 d
O6 O 0.3913(2) -0.09586(18) 0.82536(11) 0.0740(6) Uani 1 1 d
O7 O 0.4016(2) 0.4692(2) 0.63330(10) 0.0830(7) Uani 1 1 d
O8 O 0.5867(2) 0.54610(19) 0.67348(10) 0.0728(6) Uani 1 1 d
O9 O 0.57669(18) 0.51073(15) 0.89559(8) 0.0516(4) Uani 1 1 d
O10 O 0.49106(17) 0.61499(14) 0.80928(9) 0.0537(4) Uani 1 1 d
N1 N 0.48162(16) 0.20217(15) 0.77666(8) 0.0322(4) Uani 1 1 d
N2 N 0.47880(18) 0.26356(16) 0.71466(8) 0.0371(4) Uani 1 1 d
N3 N 0.39560(18) 0.03022(16) 0.70910(10) 0.0400(4) Uani 1 1 d
N4 N 0.63670(19) 0.0311(2) 0.74468(9) 0.0450(5) Uani 1 1 d
N5 N 0.4670(2) -0.00838(16) 0.83125(9) 0.0415(4) Uani 1 1 d
N6 N 0.4938(2) 0.47360(18) 0.67424(9) 0.0463(5) Uani 1 1 d
N7 N 0.52465(17) 0.51846(15) 0.83802(9) 0.0360(4) Uani 1 1 d
C1 C 0.4932(2) 0.38174(19) 0.73029(10) 0.0349(4) Uani 1 1 d
C2 C 0.50647(19) 0.40138(18) 0.80168(10) 0.0319(4) Uani 1 1 d
C3 C 0.49681(19) 0.28510(17) 0.83170(9) 0.0293(4) Uani 1 1 d
C4 C 0.4934(2) 0.07008(18) 0.76772(10) 0.0328(4) Uani 1 1 d
O1' O 0.7928(2) 0.28943(19) 1.08242(10) 0.0728(6) Uani 1 1 d
O2' O 0.67755(18) 0.44246(15) 1.03642(9) 0.0534(4) Uani 1 1 d
O3' O 0.86333(17) 0.10557(17) 0.97956(9) 0.0586(5) Uani 1 1 d
O4' O 0.66662(18) 0.04635(15) 1.01400(9) 0.0524(4) Uani 1 1 d
O5' O 0.74885(16) 0.24788(17) 0.86087(8) 0.0507(4) Uani 1 1 d
O6' O 0.85327(18) 0.38359(17) 0.92710(10) 0.0642(5) Uani 1 1 d
O7' O 0.2519(2) 0.1631(2) 1.09671(11) 0.0859(7) Uani 1 1 d
O8' O 0.1735(2) 0.33524(19) 1.05448(11) 0.0714(6) Uani 1 1 d
O9' O 0.21971(17) 0.26067(19) 0.82877(9) 0.0610(5) Uani 1 1 d
O10' O 0.11121(17) 0.23639(19) 0.92296(10) 0.0621(5) Uani 1 1 d
N1' N 0.54937(16) 0.25615(15) 0.96224(8) 0.0312(3) Uani 1 1 d
N2' N 0.47896(17) 0.24652(16) 1.02227(8) 0.0356(4) Uani 1 1 d
N3' N 0.72445(19) 0.33724(18) 1.03827(9) 0.0429(4) Uani 1 1 d
N4' N 0.74569(19) 0.12023(17) 0.99078(9) 0.0394(4) Uani 1 1 d
N5' N 0.77269(18) 0.30215(18) 0.91468(10) 0.0406(4) Uani 1 1 d
N6' N 0.25044(19) 0.24681(18) 1.05556(9) 0.0447(4) Uani 1 1 d
N7' N 0.21356(18) 0.25012(16) 0.89122(9) 0.0393(4) Uani 1 1 d
C1' C 0.3537(2) 0.24638(18) 1.00279(10) 0.0342(4) Uani 1 1 d
C2' C 0.33806(19) 0.25324(17) 0.93069(10) 0.0318(4) Uani 1 1 d
C3' C 0.46521(19) 0.26057(17) 0.90478(9) 0.0290(4) Uani 1 1 d
C4' C 0.6903(2) 0.25447(18) 0.97438(10) 0.0329(4) Uani 1 1 d
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
N2 N1 C3 112.04(15)
N2 N1 C4 111.28(15)
C3 N1 C4 135.39(16)
C1 N2 N1 104.69(16)
O1 N3 O2 128.7(2)
O1 N3 C4 117.28(18)
O2 N3 C4 114.05(17)
O4 N4 O3 128.9(2)
O4 N4 C4 116.78(19)
O3 N4 C4 114.3(2)
O6 N5 O5 128.3(2)
O6 N5 C4 117.75(19)
O5 N5 C4 113.87(17)
O8 N6 O7 126.4(2)
O8 N6 C1 116.70(18)
O7 N6 C1 116.85(19)
O10 N7 O9 125.84(18)
O10 N7 C2 118.24(17)
O9 N7 C2 115.90(16)
N2 C1 C2 112.45(17)
N2 C1 N6 118.19(18)
C2 C1 N6 129.36(18)
C3 C2 C1 106.28(17)
C3 C2 N7 125.36(17)
C1 C2 N7 128.36(18)
C2 C3 N1 104.51(16)
C2 C3 C3' 125.72(17)
N1 C3 C3' 127.07(16)
N1 C4 N5 115.30(15)
N1 C4 N3 107.99(15)
N5 C4 N3 109.46(16)
N1 C4 N4 112.03(16)
N5 C4 N4 105.17(16)
N3 C4 N4 106.53(15)
N2' N1' C3' 112.00(15)
N2' N1' C4' 112.15(15)
C3' N1' C4' 135.80(16)
C1' N2' N1' 104.86(16)
O1' N3' O2' 128.7(2)
O1' N3' C4' 116.47(18)
O2' N3' C4' 114.79(17)
O4' N4' O3' 128.92(19)
O4' N4' C4' 116.07(17)
O3' N4' C4' 114.99(17)
O6' N5' O5' 129.35(19)
O6' N5' C4' 117.06(19)
O5' N5' C4' 113.55(18)
O7' N6' O8' 125.9(2)
O7' N6' C1' 117.74(19)
O8' N6' C1' 116.29(19)
O10' N7' O9' 125.1(2)
O10' N7' C2' 117.11(18)
O9' N7' C2' 117.76(18)
N2' C1' C2' 112.19(17)
N2' C1' N6' 118.71(18)
C2' C1' N6' 128.99(19)
C3' C2' C1' 106.35(17)
C3' C2' N7' 126.52(17)
C1' C2' N7' 127.12(18)
C2' C3' N1' 104.59(15)
C2' C3' C3 125.05(17)
N1' C3' C3 129.89(17)
N1' C4' N5' 114.58(16)
N1' C4' N3' 109.07(15)
N5' C4' N3' 107.94(16)
N1' C4' N4' 113.00(16)
N5' C4' N4' 105.42(15)
N3' C4' N4' 106.39(15)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
O1 N3 1.192(2)
O2 N3 1.196(2)
O3 N4 1.200(3)
O4 N4 1.192(3)
O5 N5 1.201(2)
O6 N5 1.192(2)
O7 N6 1.197(3)
O8 N6 1.196(2)
O9 N7 1.218(2)
O10 N7 1.202(2)
N1 N2 1.360(2)
N1 C3 1.381(2)
N1 C4 1.408(2)
N2 C1 1.289(3)
N3 C4 1.533(3)
N4 C4 1.551(3)
N5 C4 1.505(3)
N6 C1 1.451(3)
N7 C2 1.429(3)
C1 C2 1.397(3)
C2 C3 1.359(3)
C3 C3' 1.473(2)
O1' N3' 1.190(2)
O2' N3' 1.202(2)
O3' N4' 1.199(2)
O4' N4' 1.197(2)
O5' N5' 1.205(2)
O6' N5' 1.193(2)
O7' N6' 1.187(3)
O8' N6' 1.204(2)
O9' N7' 1.213(2)
O10' N7' 1.202(2)
N1' N2' 1.367(2)
N1' C3' 1.375(2)
N1' C4' 1.411(3)
N2' C1' 1.289(3)
N3' C4' 1.542(3)
N4' C4' 1.548(3)
N5' C4' 1.510(3)
N6' C1' 1.456(2)
N7' C2' 1.437(3)
C1' C2' 1.399(3)
C2' C3' 1.365(3)
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
C3 N1 N2 C1 0.6(2)
C4 N1 N2 C1 -168.52(17)
N1 N2 C1 C2 0.4(2)
N1 N2 C1 N6 -179.78(17)
O8 N6 C1 N2 -127.9(2)
O7 N6 C1 N2 52.0(3)
O8 N6 C1 C2 51.9(3)
O7 N6 C1 C2 -128.2(3)
N2 C1 C2 C3 -1.2(2)
N6 C1 C2 C3 179.0(2)
N2 C1 C2 N7 179.68(19)
N6 C1 C2 N7 -0.2(4)
O10 N7 C2 C3 -157.56(19)
O9 N7 C2 C3 24.2(3)
O10 N7 C2 C1 21.4(3)
O9 N7 C2 C1 -156.9(2)
C1 C2 C3 N1 1.4(2)
N7 C2 C3 N1 -179.41(18)
C1 C2 C3 C3' -160.94(18)
N7 C2 C3 C3' 18.2(3)
N2 N1 C3 C2 -1.3(2)
C4 N1 C3 C2 164.2(2)
N2 N1 C3 C3' 160.74(18)
C4 N1 C3 C3' -33.8(3)
N2 N1 C4 N5 -167.18(16)
C3 N1 C4 N5 27.3(3)
N2 N1 C4 N3 -44.4(2)
C3 N1 C4 N3 150.0(2)
N2 N1 C4 N4 72.6(2)
C3 N1 C4 N4 -93.0(2)
O6 N5 C4 N1 130.9(2)
O5 N5 C4 N1 -52.8(2)
O6 N5 C4 N3 9.0(3)
O5 N5 C4 N3 -174.79(17)
O6 N5 C4 N4 -105.1(2)
O5 N5 C4 N4 71.1(2)
O1 N3 C4 N1 117.3(2)
O2 N3 C4 N1 -62.3(2)
O1 N3 C4 N5 -116.5(2)
O2 N3 C4 N5 64.0(2)
O1 N3 C4 N4 -3.3(2)
O2 N3 C4 N4 177.19(18)
O4 N4 C4 N1 -19.6(2)
O3 N4 C4 N1 161.59(18)
O4 N4 C4 N5 -145.56(19)
O3 N4 C4 N5 35.6(2)
O4 N4 C4 N3 98.3(2)
O3 N4 C4 N3 -80.5(2)
C3' N1' N2' C1' -0.7(2)
C4' N1' N2' C1' -178.55(16)
N1' N2' C1' C2' 1.2(2)
N1' N2' C1' N6' -175.37(16)
O7' N6' C1' N2' -57.5(3)
O8' N6' C1' N2' 120.3(2)
O7' N6' C1' C2' 126.6(3)
O8' N6' C1' C2' -55.6(3)
N2' C1' C2' C3' -1.2(2)
N6' C1' C2' C3' 174.85(19)
N2' C1' C2' N7' 177.39(18)
N6' C1' C2' N7' -6.5(3)
O10' N7' C2' C3' 176.0(2)
O9' N7' C2' C3' -3.6(3)
O10' N7' C2' C1' -2.4(3)
O9' N7' C2' C1' 178.1(2)
C1' C2' C3' N1' 0.7(2)
N7' C2' C3' N1' -177.91(17)
C1' C2' C3' C3 -172.06(17)
N7' C2' C3' C3 9.3(3)
N2' N1' C3' C2' -0.1(2)
C4' N1' C3' C2' 177.1(2)
N2' N1' C3' C3 172.24(18)
C4' N1' C3' C3 -10.6(3)
C2 C3 C3' C2' 85.2(3)
N1 C3 C3' C2' -73.2(3)
C2 C3 C3' N1' -85.7(3)
N1 C3 C3' N1' 115.9(2)
N2' N1' C4' N5' -163.07(16)
C3' N1' C4' N5' 19.8(3)
N2' N1' C4' N3' -42.0(2)
C3' N1' C4' N3' 140.9(2)
N2' N1' C4' N4' 76.15(19)
C3' N1' C4' N4' -101.0(2)
O6' N5' C4' N1' 127.3(2)
O5' N5' C4' N1' -54.8(2)
O6' N5' C4' N3' 5.6(2)
O5' N5' C4' N3' -176.53(17)
O6' N5' C4' N4' -107.8(2)
O5' N5' C4' N4' 70.1(2)
O1' N3' C4' N1' 128.4(2)
O2' N3' C4' N1' -51.5(2)
O1' N3' C4' N5' -106.5(2)
O2' N3' C4' N5' 73.5(2)
O1' N3' C4' N4' 6.3(3)
O2' N3' C4' N4' -173.72(17)
O4' N4' C4' N1' -24.3(2)
O3' N4' C4' N1' 157.01(17)
O4' N4' C4' N5' -150.21(18)
O3' N4' C4' N5' 31.2(2)
O4' N4' C4' N3' 95.3(2)
O3' N4' C4' N3' -83.3(2)
